| Abstract|| |
Aim: The aim of this systematic review was to compare the effect of body temperature (I) on the cyclic fatigue resistance (O) of nickel–titanium (NiTi) endodontic instruments (P) to that of room temperature (C).
Methods: The study was registered in the PROSPERO database (CRD42020204286). A systematic search in PubMed, Scopus, Web of Science, Google Scholar, and OpenGrey was conducted in English until December 31, 2021. In vitro studies comparing the cyclic fatigue resistance of NiTi instruments at the body (35°C ± 2°C) and room temperature (20°C–25°C) were included. Eligible studies were evaluated for risk of bias and meta-analyzed to estimate the effects.
Results: Twenty-one studies out of 347 met the criteria for inclusion. The meta-analysis included six studies (n = 215) with comparative study parameters. The overall effect sizes (5.49; 95% confidence interval [CI]: 4.04–6.93) were significantly different (P < 0.001), indicating that the mean values at room temperature were significantly (P < 0.001) higher. The effect sizes for full rotary motion (standardized mean difference [SMD]: 4.80; 95% CI: 3.04–6.56) and reciprocating motion (SMD: 6.37; 95% CI: 3.63–9.11) were not significantly different (P = 0.346). Heterogeneity was high (I2 = 94%). Sensitivity analysis revealed that the SMD values were not significantly different (P > 0.05) from the overall effect size, indicating that none of the studies had an effect on the overall effect size.
Conclusions: Within the limitation of the study, the cyclic fatigue resistance of heat-treated NiTi endodontic files is significantly reduced at body temperature when compared to room temperature. Cyclic fatigue testing should be conducted at simulated body temperature.
Keywords: Cyclic fatigue; dental instrument; endodontics; meta-analysis; nickel–titanium; root canal preparation/instrumentation; root canal therapy/instrumentation; temperature
|How to cite this article:|
Savitha S, Sharma S, Kumar V, Chawla A, Vanamail P, Logani A. Effect of body temperature on the cyclic fatigue resistance of the nickel”titanium endodontic instruments: A systematic review and meta-analysis of in vitro studies. J Conserv Dent 2022;25:338-46
|How to cite this URL:|
Savitha S, Sharma S, Kumar V, Chawla A, Vanamail P, Logani A. Effect of body temperature on the cyclic fatigue resistance of the nickel”titanium endodontic instruments: A systematic review and meta-analysis of in vitro studies. J Conserv Dent [serial online] 2022 [cited 2022 Oct 3];25:338-46. Available from: https://www.jcd.org.in/text.asp?2022/25/4/338/353149
| Introduction|| |
Nickel–titanium (NiTi) engine-driven instruments continue to be the mainstay in performing mechanical debridement and shaping during endodontic treatment. It has revolutionized the root canal preparation technique by decreasing operator fatigue, time, and procedural errors associated with manual instrumentation. Despite the increased flexibility, a major concern related to their use is the possibility of intracanal separation. The reported incidence of separation is in the wide range of 0.4%–23%. This is widely attributed to two mechanisms. One is torsional fatigue which occurs when the file's tip is locked inside the canal while the main body or shaft of the file continues to rotate, exceeding the elastic limit. The second is cyclic fatigue, which results from rotation around a curve with the consequence of repeated tension and compression of metal and, finally, work hardening followed by fracture. Cyclic or flexural fatigue accounts for most fractured instruments during clinical use and has been studied extensively. The various factors affecting the cyclic fatigue of a NiTi instrument include the instrument design, type of alloy, radius of curvature, angle of curvature, movement kinematics, and temperature. Environmental or intracanal or body temperature is an important confounding factor that is least studied. It is relevant since the metallurgy of NiTi alloys exhibits different behaviors at room or body temperature. Earlier, most of the fatigue studies were performed at room temperature. Recently, many studies have reported the dramatic effect of body temperature on the cyclic fatigue resistance of NiTi instruments with a reported 300%–500% impact on their lifetime.,,, Hence, the present systematic review aimed to evaluate the effect of body temperature on the cyclic fatigue resistance of the NiTi endodontic instruments compared to room temperature. The objective was to determine how temperature affects the cyclic fatigue resistance of NiTi instruments and help the clinicians to learn more about the mechanical behavior of NiTi in clinical situations.
| Methods|| |
Protocol and registration
The current review followed the Preferred Reporting Items for Systematic Reviews and Meta-Analyses 2020 guidelines. The review protocol was registered a priori in the PROSPERO database (CRD42020204286).
Research question and eligibility criteria
The PICOS acronym was used to devise the following question: What is the effect of body temperature (I) on the cyclic fatigue resistance (O) of NiTi endodontic instruments (P) when compared to room temperature (C) as measured by in vitro studies (S)?
- Population: NiTi endodontic instruments
- Intervention: Body temperature (35°C ± 2°C)
- Comparison: Room temperature (20°C–25°C).
- Outcomes: Cyclic fatigue resistance, i.e., the number of cycles to fracture (NCF) or time to fracture (TTF).
- Studies: In vitro studies.
Exclusion criteria included studies assessing cyclic fatigue resistance at temperatures other than those indicated above. In addition, abstracts, conference proceedings, reviews, and studies published in languages other than English were not selected. However, those translated into English were included.
Information sources, search strategy, and selection process
A search of the literature was conducted in three databases: PubMed (1964–2021), Scopus (1960–2021), and Web of Science (1980–2021) until December 31, 2021. Google Scholar (first 100 returns) and OpenGrey databases were searched electronically for unpublished manuscripts, research reports, doctoral dissertations, and other gray literature. The electronic search strategy was developed using the most cited descriptors in previous publications on this theme combining Medical Subject Heading terms and text words. For the database, the following terms were combined: “Body temperature,” “Temperature,” “Environmental temperature,” “Fatigue,” “Cyclic fatigue,” “Fatigue resistance,” “Flexural fatigue,” “Fracture resistance,” “Nickel titanium,” “Niti,” “Nitinol,” “Dental instruments,” “instrument,” and “Rotary.” The Boolean operators “AND” and “OR” were applied to combine the terms and create a search strategy. The search strategies for each database are summarized in [Supplementary Table 1]. The search was expanded to include reference lists for screened studies and published reviews. The leading endodontic journals, including the Journal of Endodontics, the International Endodontic Journal, and the Australian Endodontic Journal, were manually searched. Duplicate articles were removed from the database using the Covidence tool (Melbourne, Australia). The selection of studies was performed using a two-stage screening process. This was accomplished by two independent reviewers (SS1 and SS2) screening the title and abstract for appropriate studies and reading the full text. The reasons for exclusion are documented in [Supplementary Table 2].,,,, In the event of a disagreement, a third reviewer (AL) was consulted.
Data collection and data items
The following data were recorded in an Excel spreadsheet (Microsoft, Redmond, WA, USA) by the two independent reviewers: author, year of publication, instrument name, size, taper, type of alloy (conventional or heat-treated), sample size, motion type (full rotary or reciprocating), testing model (static or dynamic), angle of curvature, radius of curvature, distance from the tip, immersion media, rotational speed, insertion depth, insertion angle, material of artificial canal, inner diameter of the canal, and NCF or TTF at room and body temperatures [Table 1].
Study risk of bias assessment
The methodological quality of the included research was determined using an adaption of a prior systematic review that included in vitro investigations. The domains listed below were used: (1) sample standardization, (2) sample size calculation, (3) sample randomization, (4) single-operator, (5) blinding, (6) testing model standardization, and (7) appropriate statistical analysis. The domains were categorized as “+” to specify a low risk of bias (RoB) and “-” to indicate a high RoB. The articles were classed as having a low RoB if they had six or more domains classified as low (+), a moderate RoB if four or five domains were classified as low, and a high RoB if only three or fewer domains were classified as low. The two reviewers independently assessed the quality (SS1 and SS2). In a disagreement, a third reviewer (AL) was consulted.
| Results|| |
[Figure 1] presents a flowchart of the systematic review process. A total of 21 studies met the criteria for inclusion.,,,,,,,,,,,,,,,,,,,,
|Figure 1: The PRISMA flow diagram. PRISMA: Preferred Reporting Items for Systematic Reviews and Meta-Analyses|
Click here to view
Characteristics of instrument types
The studies examined a total of 29 instruments, nine of which were made of conventional NiTi alloy and eight of which were reciprocating systems. The size of the instrument tip ranged from #20 to #40; however, the majority of studies utilized size #25. In addition, the taper and speed of rotation varied between studies [Table 1].
Characteristics of study design
The studies revealed differences in the test model type, radius of curvature, angle of curvature, and immersion media.,,,,,,,,,,,,,,,,,,,, The distance of the curvature from the tip, the fit of the instrument, angle of insertion, and length of the instrument inserted were not mentioned in all the studies [Table 1].
Risk of bias in studies
[Table 2] contains a detailed information addressing the RoB in the selected studies. The RoB was evaluated as moderate to high overall.
Because of the heterogeneity among the study design and instrument types, it was decided not to perform a meta-analysis on overall data. To ensure homogeneity, the meta-analysis included only those studies that matched the following criteria:
- Heat-treated files
- Tip size of 25
- Static stainless steel model
- Angle of curvature = 60°
- Radius of curvature = 5 mm
- Water as an immersion media
- Cyclic fatigue expressed in NCF.
Six studies were included,,,,,, examining 10 different instrument types, including the ProTaper Gold (Dentsply Sirona, Charlotte, NC, USA), EdgeFile (EdgeEndo, Albuquerque, NM), Vortex Blue (Dentsply Sirona, Charlotte, NC, USA), Reciproc Blue (VDW, Munich, Germany), HyFlex EDM (Coltene, Cuyahoga Falls, OH, USA), WaveOne Gold (Dentsply Sirona, Charlotte, NC, USA), Twisted File Adaptive (TFA) (SybronEndo, CA, USA), X1 Blue (MK Life, Porto Alegre, RS, Brazil), 2Shape (MicroMega, Besancon, France), and One Curve (MicroMega, Besancon, France). Three of these systems were reciprocating while one had an adaptive (rotation–reciprocating) motion. The TFA changes to a reciprocating mode when engaging dentin or stress. As a result, it was considered under reciprocating subgroup during the meta-analysis [Table 1].
STATA version 16.0 (Stata Corp, College Station, Texas, 77845, USA) software was used to carry the meta-analysis to assess whether the mean differences at 20°C and 37°C across the studies were statistically significant. The standardized mean difference (SMD) was calculated using Hedges' g bias correction and was taken as effect size with 95% confidence interval (CI). The fixed-effect model using the inverse-variance method and the random-effect model using the restricted maximum likelihood method were estimated. The heterogeneity was tested across the studies using the I2-statistics using DerSimonian–Laird estimator for tau2. I2-statistics of >50% was considered as significant heterogeneity. The publication bias was assessed using the funnel plot and Begg–Egger regression test. Since two motions (rotary and reciprocating) were adopted, a subgroup analysis was carried out. To assess the consistency of the results, sensitivity analysis was performed by the method of leaving one out study. A meta-regression of SMD on the other study variables available was performed to find out significant contributing factors.
Results of the meta-analysis
Fourteen groups (8 groups with rotary motion and 6 groups with reciprocating motion) were evaluated in six studies with two arms (20°–25°C and 35 ± 2°C). A total of 215 instruments per arm consisting of 140 with rotary motion and 75 with reciprocating motion were studied. All the 14 groups demonstrated that the effect sizes were significantly different, indicating that the SMD was significantly (P < 0.001) higher in the 20°C arm [Figure 1]. The overall effect size for the fixed-effect model was 2.99 (95% CI: 2.66–3.33) and for the random-effect model was 5.49 (95% CI: 4.04–6.93) [Figure 2].
|Figure 2: Forest plot analysis comparing the NCF values at room and body temperatures. The subgroups represent different motion kinematics (Motion code 0 = Rotary, Motion code 1 = Reciprocating). NCF: Number of cycles to fracture|
Click here to view
Heterogeneity (I2-statistics = 94%) was very high, and it was highly significant (P < 0.001) between the studies. Since the heterogeneity was more than the threshold level (50%), subsequent analyses were restricted to the random-effect model. Subgroup analysis by motion showed that the overall effect size for full rotary motion (SMD: 4.80; 95% CI: 3.04–6.56) and reciprocating motion (SMD: 6.37; 95% CI: 3.63–9.11) did not differ significantly (P = 0.346) [Figure 2]. Sensitivity analysis by leaving out one study was carried out to determine the influence of any particular study on the outcome [Supplementary Table 3]. The SMD values did not differ significantly (P > 0.05) from the overall effect size by leaving one particular study, confirming that none of the studies influenced the overall effect size.
Funnel plot analysis indicated the presence of high publication bias as evident by an asymmetric pattern of the effective size. Further, the intercept of the Begg–Egger regression was highly significant (P < 0.001), confirming the presence of publication bias [Supplementary Figure 1]. To assess the possible influencing factors for the high heterogeneity level, a meta-regression analysis was carried out by considering the taper size as the covariate. The testing of the regression coefficient of taper size was not statistically significant (P = 0.461), implying that the taper size was not a significant influencing factor toward the high heterogeneity level.
| Discussion|| |
The relative proportion and characteristic of the microstructural phases in a NiTi instrument determine its mechanical behavior. The alloy can be classified into two distinct temperature-dependent crystallographic phases: martensite (low-temperature phase) and austenite (high temperature or parent phase), each with its own distinct set of properties. When heated, martensite NiTi transforms into austenite. The austenite start temperature is when this phenomenon begins (As). The temperature at which it is complete is referred to as the austenite finish temperature (Af). When austenite NiTi is cooled to a specific temperature, it transforms into martensite. Similarly, martensite start temperature (Ms) and martensite finish temperature (Mf) exist. The transformation temperatures have a substantial effect on the mechanical characteristics and behavior of NiTi, which can be varied during the production process by minor compositional changes, impurity additions, and heat treatments. The Af temperature of the conventional NiTi files is near or below room temperature. In contrast, the Af temperature of the vast majority of heat-treated files is clearly above body temperature. CM wire, M-wire, and conventional SE NiTi wire have an Af of approximately 55°C, 50°C, and 16°–31°C, respectively. During root canal preparation, the average intracanal temperature is 35.1°C, comparable to body temperature. Thus, conventional NiTi files are predominantly in the austenite phase at or below intracanal temperature, whereas heat-treated files are predominantly in the martensite/R-phase/hybrid phase at intracanal temperature.
The bulk material properties primarily determine fatigue life. A hybrid (austenite–martensite) microstructure containing a trace of martensite is more likely to be fatigue resistant than a completely austenitic microstructure. This is often explained by martensite's stronger resistance to fatigue crack growth than stable austenite. The fatigue crack propagation speed of austenitic structures is significantly faster than that of martensite structures at the same stress intensity level. In addition, due to the energy absorption properties of its twinned phase structure, the martensitic phase transformation exhibits exceptional damping characteristics.
In cyclic fatigue studies, environmental temperature is a crucial confounding variable. Numerous investigations have established a considerable effect of ambient temperature on the cyclic fatigue resistance of NiTi endodontic instruments since NiTi alloys behave differently depending on their metallurgical properties.,,, Thus, compared to room temperature, the current systematic review studied the influence of body temperature on the cyclic fatigue resistance of NiTi devices. The studies that examined the effect of various temperatures (−20°C to 60°C) were excluded, as cooled or heated irrigant solutions rapidly equilibrate to body temperature inside the root canal. The included 21 studies demonstrated notable heterogeneity in the test model type, curvature radius, angle of curvature, immersion media, and instrument features. The present review demonstrates the importance of developing an international standard for validating a device for cyclic fatigue testing of NiTi rotary endodontic instruments. In an ideal scenario, it would enable the testing of all instruments with a precise trajectory in terms of radius and angle of curvature, fit, and angle of insertion, among other characteristics, allowing the comparison of different instruments.
Six studies were selected with similar study designs, instrument characteristics, and outcome measures to achieve homogeneity.,,,,, A meta-analysis was performed, which discovered that the cyclic fatigue resistance of heat-treated NiTi endodontic instruments is significantly reduced at body temperature. This can be attributed to the alloy transitioning to the austenitic phase in heat-treated instruments. At room temperature, the various heat-treated files are martensitic and transform to a more austenitic state at body temperature, resulting in a mixed martensitic, R-phase, and austenitic structure. The martensitic to austenitic conversion is not complete at body temperature, but a considerable proportion is already austenitic. However, the crystal lattice of conventional NiTi instruments is almost identical at room and body temperatures; nevertheless, literature reports that fatigue resistance is reduced, albeit slightly. This implies that additional unidentified factors may play a role that warrants further investigation. In addition to alloy, the cyclic fatigue of an endodontic instrument is also affected by the instrument's working kinematics (rotary and reciprocating) and diameter., Hence, a subgroup analysis was conducted using the motion type. Even though the effect size for the reciprocating motion was higher than the rotary motion, the difference was not statistically significant.
The primary limitation of this meta-analysis was the high degree of heterogeneity attributed to the different instrument brands and designs. The instruments all had the same tip size (#25). However, the tapers ranged from 2% to 8%. Previous research has demonstrated that instruments with a narrower taper exhibit greater cyclic fatigue resistance. As a result, the taper size was tested as a covariate in a meta-regression analysis and found to have no significant effect on the effect size, implying that other variables may have contributed to the high heterogeneity. Each of the heat-treated alloys included in the meta-analysis has a different phase transformation temperature, contributing to the heterogeneity. Given that temperature is the focus of the included studies, the methods used to maintain the temperature during testing varied widely, including using a thermocouple or a hotplate and ice. Again, various study design parameters such as the distance of curvature from the tip, the instrument's fit, and the angle of insertion were not mentioned in all studies and could not be retrieved. In addition, most studies demonstrated a high or moderate RoB. Sensitivity analysis was used to determine the effect of omitting one study on the outcome. However, none of the studies affected the overall effect size. High publication bias was also a limitation, indicating that there may be a bias toward publishing only positive effects or due to language bias.
The current review's strength was that, despite discovering significant variation in cyclic fatigue testing models, it attempted a meta-analysis by including studies with comparable parameters. In this regard, this is the first systematic review to investigate the effect of body temperature on the cyclic fatigue resistance of NiTi endodontic instruments.
| Conclusions|| |
Within the limitations of this systematic review, the overall effect size was significantly higher at room temperature, indicating that the cycle fatigue resistance of heat treated NiTi instruments decreases significantly at body temperature compared to room temperature. As a result, future cyclic fatigue testing should be performed at a simulated body temperature that resembles the intracanal environment.
Financial support and sponsorship
Conflicts of interest
There are no conflicts of interest.
| References|| |
Cecchin D, de Sousa-Neto MD, Pécora JD, Gariba-Silva R. Cutting efficiency of four different rotary nickel: Titanium instruments. J Conserv Dent 2011;14:117-9.
] [Full text]
Cheung GS. Instrument fracture: Mechanisms, removal of fragments, and clinical outcomes. Endod Top 2007;16:1-26.
Hülsmann M, Donnermeyer D, Schäfer E. A critical appraisal of studies on cyclic fatigue resistance of engine-driven endodontic instruments. Int Endod J 2019;52:1427-45.
Plotino G, Grande NM, Cordaro M, Testarelli L, Gambarini G. A review of cyclic fatigue testing of nickel-titanium rotary instruments. J Endod 2009;35:1469-76.
Cheung GS, Peng B, Bian Z, Shen Y, Darvell BW. Defects in ProTaper S1 instruments after clinical use: Fractographic examination. Int Endod J 2005;38:802-9.
Schäfer E, Bürklein S, Donnermeyer D. A critical analysis of research methods and experimental models to study the physical properties of NiTi instruments and their fracture characteristics. Int Endod J 2022;55 Suppl 1:72-94.
Zupanc J, Vahdat-Pajouh N, Schäfer E. New thermomechanically treated NiTi alloys - A review. Int Endod J 2018;51:1088-103.
Grande NM, Plotino G, Silla E, Pedullà E, DeDeus G, Gambarini G, et al.
Environmental temperature drastically affect flexural fatigue resistance of nickel-titanium rotary files. J Endod 2017;43:1157-60.
Shen Y, Huang X, Wang Z, Wei X, Haapasalo M. Low environmental temperature influences the fatigue resistance of nickel-titanium files. J Endod 2018;44:626-9.
Yılmaz K, Uslu G, Gündoğar M, Özyürek T, Grande NM, Plotino G. Cyclic fatigue resistances of several nickel-titanium glide path rotary and reciprocating instruments at body temperature. Int Endod J 2018;51:924-30.
Arslan H, Doğanay Yıldız E, Taş G, Karataş E, Tepecik E. Effects of continuous irrigation at room temperature or +4°C on the cyclic fatigue resistance of K3XF instruments. J Dent Res Dent Clin Dent Prospects 2020;14:153-7.
Page MJ, McKenzie JE, Bossuyt PM, Boutron I, Hoffmann TC, Mulrow CD, et al.
The PRISMA 2020 statement: An updated guideline for reporting systematic reviews. BMJ 2021;372:n71.
Silva EJ, Zanon M, Hecksher F, Belladonna FG, de Vasconcelos RA, Fidalgo TK. Influence of autoclave sterilization procedures on the cyclic fatigue resistance of heat-treated nickel-titanium instruments: A systematic review. Restor Dent Endod 2020;45:e25.
Arias A, Hejlawy S, Murphy S, de la Macorra JC, Govindjee S, Peters OA. Variable impact by ambient temperature on fatigue resistance of heat-treated nickel titanium instruments. Clin Oral Investig 2019;23:1101-8.
Arias A, Macorra JC, Govindjee S, Peters OA. Correlation between temperature-dependent fatigue resistance and differential scanning calorimetry analysis for 2 contemporary rotary instruments. J Endod 2018;44:630-4.
Cardoso RM, Carvalho Alves NC, de Menezes SE, Batista SM, Vieira TM, Elgarten Rocha GN, et al.
Influence of temperature on the cyclic fatigue of nickel-titanium instruments with different heat treatments on severely curved canals. J Contemp Dent Pract 2019;20:697-701.
de Vasconcelos RA, Murphy S, Carvalho CA, Govindjee RG, Govindjee S, Peters OA. Evidence for reduced fatigue resistance of contemporary rotary instruments exposed to body temperature. J Endod 2016;42:782-7.
Generali L, Malovo A, Bolelli G, Borghi A, La Rosa GR, Puddu P, et al.
Mechanical properties and metallurgical features of new green NiTi reciprocating instruments. Materials (Basel) 2020;13:E3736.
Huang X, Shen Y, Wei X, Haapasalo M. Fatigue resistance of nickel-titanium instruments exposed to high-concentration hypochlorite. J Endod 2017;43:1847-51.
Ismail AG, Galal M, Nagy MM. Effect of different kinematics and operational temperature on cyclic fatigue resistance of rotary NiTi systems. Bull Natl Res Cent 2020;44:116.
Keleş A, Eymirli A, Uyanık O, Nagas E. Influence of static and dynamic cyclic fatigue tests on the lifespan of four reciprocating systems at different temperatures. Int Endod J 2019;52:880-6.
La Rosa GR, Palermo C, Ferlito S, Isola G, Indelicato F, Pedullá E. Influence of surrounding temperature and angle of file access on cyclic fatigue resistance of two single file nickel-titanium instruments. Aust Endod J 2021;47:260-4.
La Rosa GR, Shumakova V, Isola G, Indelicato F, Bugea C, Pedullá E. Evaluation of the cyclic fatigue of two single files at body and room temperature with different radii of curvature. Materials (Basel) 2021;14:2256.
Plotino G, Grande NM, Mercadé Bellido M, Testarelli L, Gambarini G. Influence of temperature on cyclic fatigue resistance of ProTaper Gold and ProTaper universal rotary files. J Endod 2017;43:200-2.
Plotino G, Grande NM, Testarelli L, Gambarini G, Castagnola R, Rossetti A, et al.
Cyclic fatigue of reciproc and reciproc blue nickel-titanium reciprocating files at different environmental temperatures. J Endod 2018;44:1549-52.
Topçuoğlu HS, Topçuoğlu G, Kafdağ Ö, Balkaya H. Effect of two different temperatures on resistance to cyclic fatigue of one Curve, EdgeFile, HyFlex CM and ProTaper next files. Aust Endod J 2020;46:68-72.
Vieira TM, Alves NC, de Andrade Silva S, de Almeida AC, Telles CT, Albuquerque DS. Influence of temperature on the cyclic fatigue resistance of reciproc blue instruments. J Contemp Dent Pract 2020;21:277-9.
Vieira TM, Cardoso RM, Alves NC, Emanuel Acioly Conrado de Menezes S, Batista SM, Silva SA, et al.
Cyclic fatigue resistance of blue heat-treated instruments at different temperatures. Int J Biomater 2021;2021:5584766.
Dosanjh A, Paurazas S, Askar M. The effect of temperature on cyclic fatigue of nickel-titanium rotary endodontic instruments. J Endod 2017;43:823-6.
Alfawaz H, Alqedairi A, Alsharekh H, Almuzaini E, Alzahrani S, Jamleh A. Effects of sodium hypochlorite concentration and temperature on the cyclic fatigue resistance of heat-treated nickel-titanium rotary instruments. J Endod 2018;44:1563-6.
Gündoğar M, Özyürek T, Yılmaz K, Uslu G. Cyclic fatigue resistance of HyFlex EDM, Reciproc Blue, WaveOne Gold, and Twisted File Adaptive rotary files under different temperatures and ambient conditions. J Dent Res Dent Clin Dent Prospects 2019;13:166-71.
Klymus ME, Alcalde MP, Vivan RR, Só MV, de Vasconselos BC, Duarte MA. Effect of temperature on the cyclic fatigue resistance of thermally treated reciprocating instruments. Clin Oral Investig 2019;23:3047-52.
Saeed DH, Rafea FA. Evaluation of the effect of temperature on cyclic fatigue resistance of three types of Nickel-Titanium rotary files with various alloy properties: An in vitro
study. Erbil Dental J 2019;2:157-63.
Staffoli S, Grande NM, Plotino G, Özyürek T, Gündoğar M, Fortunato L, et al.
Influence of environmental temperature, heat-treatment and design on the cyclic fatigue resistance of three generations of a single-file nickel-titanium rotary instrument. Odontology 2019;107:301-7.
Shen Y, Zhou H, Campbell L, Wang Z, Wang R, Du T, et al.
Fatigue and nanomechanical properties of K3XF nickel-titanium instruments. Int Endod J 2014;47:1160-7.
Shen Y, Zhou HM, Zheng YF, Peng B, Haapasalo M. Current challenges and concepts of the thermomechanical treatment of nickel-titanium instruments. J Endod 2013;39:163-72.
Yoneyama T, Kobayashi C. Endodontic instruments for root canal treatment using Ti-Ni shape memory alloys. In: Yoneyama T, Miyazaki S, editors. Shape Memory Alloys for Biomedical Applications. Cambridge: Woodhead Publishing Limited; 2009. p. 297-305.
de Hemptinne F, Slaus G, Vandendael M, Jacquet W, De Moor RJ, Bottenberg P. In vivo
intracanal temperature evolution during endodontic treatment after the injection of room temperature or preheated sodium hypochlorite. J Endod 2015;41:1112-5.
McKelvey AL, Ritchie RO. Fatigue-crack growth behavior in the superelastic and shape-memory material nitinol. Metall Mater Trans A 2001;32A:731-43.
Çapar ID, Arslan H. A review of instrumentation kinematics of engine-driven nickel-titanium instruments. Int Endod J 2016;49:119-35.
Serafin M, Biasi M, Franco V, Generali L, Angerame D. Influence of different motions on the cyclic fatigue resistance of Reciproc and Reciproc Blue endodontic instruments. J Conserv Dent 2019;22:449-53. [Full text]
Elsewify TM, Saber SM, Plotino G. Cyclic fatigue resistance of three heat-Treated nickel-Titanium instruments at simulated body temperature. Saudi Endod J 2020;10:131-6. [Full text]
Shen Y, Qian W, Abtin H, Gao Y, Haapasalo M. Effect of environment on fatigue failure of controlled memory wire nickel-titanium rotary instruments. J Endod 2012;38:376-80.
Keskin C, Sivas Yilmaz Ö, Keleş A, Inan U. Comparison of cyclic fatigue resistance of Rotate instrument with reciprocating and continuous rotary nickel-titanium instruments at body temperature in relation to their transformation temperatures. Clin Oral Investig 2021;25:151-7.
Scott R, Arias A, Macorra JC, Govindjee S, Peters OA. Resistance to cyclic fatigue of reciprocating instruments determined at body temperature and phase transformation analysis. Aust Endod J 2019;45:400-6.
Alghamdi S, Huang X, Haapasalo M, Mobuchon C, Hieawy A, Hu J, et al.
Effect of curvature location on fatigue resistance of five nickel-titanium files determined at body temperature. J Endod 2020;46:1682-8.
Dr. Sidhartha Sharma
Room No 306, Division of Conservative Dentistry and Endodontics, Centre for Dental Education and Research, All India Institute of Medical Sciences, Ansarinagar, New Delhi - 110 029
Source of Support: None, Conflict of Interest: None
[Figure 1], [Figure 2]
[Table 1], [Table 2]